3d−4f Coordination Polymers Containing Alternating EE/EO Azido Chain Synthesized by Synergistic Coordination of Lanthanide and Transition Metal Ions
Hu, Xin; Zeng, Yong-Fei; Chen, Zhuo; Sañudo, E. C.; Liu, Fu-Chen; Ribas, J.; Bu, Xian-He; Crystal Growth & Design 9 (2009) 421–; doi:10.1021/cg8006475

data_4509009
_publ_section_title
;
 3d&#x2212;4f Coordination Polymers Containing Alternating EE/EO Azido
 Chain Synthesized by Synergistic Coordination of Lanthanide and
 Transition Metal Ions
;
_journal_issue                   1
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              421
_journal_paper_doi               10.1021/cg8006475
_journal_volume                  9
_journal_year                    2009
_chemical_formula_sum            'C30 H20 Eu N11 Ni2 O15'
_chemical_formula_weight         1043.92
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yn'
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 95.508(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   8.1978(8)
_cell_length_b                   26.866(3)
_cell_length_c                   16.9079(16)
_cell_measurement_temperature    293(2)
_cell_volume                     3706.6(7)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0343
_diffrn_reflns_av_sigmaI/netI    0.0414
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -10
_diffrn_reflns_limit_k_max       33
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            20817
_diffrn_reflns_theta_full        26.40
_diffrn_reflns_theta_max         26.40
_diffrn_reflns_theta_min         1.43
_exptl_absorpt_coefficient_mu    2.763
_exptl_absorpt_correction_T_max  0.6662
_exptl_absorpt_correction_T_min  0.5816
_exptl_crystal_density_diffrn    1.871
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             2064
_exptl_crystal_size_max          0.22
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.16
_refine_diff_density_max         0.826
_refine_diff_density_min         -0.643
_refine_diff_density_rms         0.103
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     612
_refine_ls_number_reflns         7591
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.041
_refine_ls_R_factor_all          0.0430
_refine_ls_R_factor_gt           0.0296
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0283P)^2^+3.6848P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0658
_refine_ls_wR_factor_ref         0.0701
_reflns_number_gt                6144
_reflns_number_total             7591
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cg8006475sup1.cif
_cod_data_source_block           3
_cod_original_cell_volume        3706.7(6)
_cod_original_formula_sum        'C30 H20 Eu1 N11 Ni2 O15'
_cod_database_code               4509009